1.1 This test method covers (1) the determination of mass gain, and (2) the surface inspection of products of zirconium, hafnium, and their alloys when corrosion tested in water at 680°F or in steam at 750°F.
1.2 This test method is to be utilized in its entirety to the extent specified herein as a product acceptance test.
1.3 This test method may be used on wrought products, castings, powder metallurgy products, and weld metals.
1.4 A complete metric companion to this test method has been developed, Test Method G 2M. Therefore, no metric equivalents are shown. However, since the mass gain and surface area of the specimen and the electrical resistivity of water are always measured or calculated in SI units, these are given in SI units.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. For specific precautionary statements, see Section 9.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D888 Test Methods for Dissolved Oxygen in Water
E29 Practice for Using Significant Digits in Test Data to Determine Conformance with Specifications
mass gain; steam corrosion; water corrosion: Aqueous corrosion testing; Corrosion--nuclear applications; Corrosivity--water; Hafnium; Nuclear applications/materials--zirconium/zirconium alloys; Steam; UNS R60001 (Zr/Zr alloy for nuclear applications); UNS R60702 (Zr/Zr alloy for nonnuclear applications); UNS R60703 (Zr/Zr alloy for nonnuclear applications); UNS R60704 (Zr/Zr alloy for nonnuclear applications); UNS R60705 (Zr/Zr alloy for nonnuclear applications); UNS R60802 (Zr/Zr alloy for nuclear applications); UNS R60804 (Zr/Zr alloy for nuclear applications); UNS R60901 (Zr/Zr alloy for nuclear applications); Water corrosivity; Zirconium/zirconium alloys--nonnuclear applications; Zirconium alloys (for nuclear applications)--specifications;
ICS Number Code 77.060 (Corrosion of metals); 77.120.99 (Other non-ferrous metals and their alloys)
ASTM International is a member of CrossRef.
Citing ASTM Standards
[Back to Top]